Abstract
Magnetsuperconductor hybrid (MSH) systems represent promising platforms to host Majorana zero modes (MZMs), the elemental building blocks for faulttolerant quantum computers. Theoretical description of such MSH structures is mostly based on simplified models, not accounting for the complexity of real materials. Here, based on density functional theory, we derive a superconducting 80band model to study an MSH system consisting of a magnetic manganese chain on the s wave superconductor niobium. For a wide range of values of the superconducting order parameter, the system is a topological superconductor, with MZMs exhibiting nonuniversal spatial patterns and a drastic accumulation of spectral weight on both sides along the magnetic chain. These side feature states can be explained by an effective model which is guided by the ab initio results. Performing scanning tunneling spectroscopy experiments on the same system, we observe a spatial structure in the lowenergy local density of states that is consistent with the theoretical findings. Our results open a firstprinciple approach to the discovery of topological superconductors.
Similar content being viewed by others
Introduction
Topological superconductors are amongst the most desirable materials, as their quasiparticles at zero energy, known as Majorana zero modes (MZMs)^{1,2,3,4}, exhibit nonAbelian braiding statistics^{5}. These MZMs are promising candidates for topological qubits^{6} and for nextgeneration quantum computing devices. Magnetsuperconductor hybrid (MSH) systems^{7,8,9,10,11,12} offer a particularly appealing platform: (i) they are comprised of wellunderstood components, magnetic atoms such as Mn, Fe, or Co deposited on the surface of a conventional superconductor such as Nb, Re or Pb; (ii) by virtue of singleatom manipulation techniques the magnetic structures can be assembled on the atomic level; (iii) scanning tunneling methods allow the local measurement and manipulation of such structures. Despite the tremendous progress, both experimentally and theoretically, in the past years, onedimensional MSH structures^{13,14,15,16,17,18,19,20}, i.e., magnetic chains on the surface of superconductors with spin–orbit coupling due to the inversionsymmetry breaking at that surface, still struggle with either sample quality or the size of the spectral gap necessary to separate the MZMs from the lowlying excited states. On the theoretical side, most simulations are (i) based on simplified models^{7,9,21,22,23} and (ii) often done for entirely onedimensional structures^{7,21}, thus ignoring the complexity and the two or threedimensional character of the materials involved. In addition, such models often couple both the magnetic Zeeman field (accounting for the magnetic moments) and the superconducting order parameter (accounting for the superconducting proximity effect) to the same orbitals, which is unphysical. Despite these simplifications, such models clearly show topological phases with localized MZMs at chain ends. Early experiments for Fe chains on Pb(110)^{13} seemed to be in good agreement with such modeling. Subsequent experiments on Fe/Pb(110) revealed a peculiar double eye feature^{24}, which was explained by the authors of ref. ^{24} through the interplay of a local suppression of the order parameter in the vicinity of the magnetic chain and the tunneling geometry, including the tip trajectory. However, the aforementioned simplified models in the literature cannot capture features such as the double eye. In the experimental part of this paper, we present dI/dV scanning tunneling spectroscopy data for Mn/Nb(110) and Fe/Nb(110) systems where characteristic lowenergy states are present on the sides of the magnetic chain. We perform ab initio modeling of Mn chains along [001] on Nb(110). We construct an effective superconducting 80band Bogoliubovde Gennes model, which turns out to be topologically nontrivial for most of the considered parameter range of the superconducting order parameter. Analysis of this model guides us to construct a further simplified model–still containing a fouratomic unit cell and a nontrivial amount of hoppings beyond nearestneighborswhere the zeroenergy states for the topological phase exhibit sidefeatures. Further investigation of this model reveals that the spatial structure of the emerging MZMs sensitively depends on the size of the spectral gap, with lowenergy features varying between localized along the side of the magnetic chains and localized near the end, with the latter resembling the previously observed doubleeye feature. Due to the promising agreement of the modeling with our scanning tunneling experiments for Mn chains on Nb(110) and the similarities to other MSH structures, such as Fe chains on Nb(110) or Pb(110), our work questions the notion of pointlike MZMs as the hallmark of onedimensional topological superconductors. We furthermore propose that MZMs appearing as side features might be a common property of topologically nontrivial MSH structures in the small gap regime due to the complex interplay of the MZM’s orbital composition and their repulsion from the magnetic chain.
Results
DFT modeling
Using density functional theory (DFT) and projective Wannier functions, we study the electronic structure of Mn chains on Nb(110), and map it onto a tightbinding model to extract the orbital dependence, spin splitting, and spin–orbit coupling. To this end, we construct a slab supercell for the Mn chains along the [001] direction with d_{Mn−Mn} = 3.30 Å on Nb(110). There is little previous work on ab initiobased modeling of MSH structures, see refs. ^{25,26} for two notable exceptions. Figure 1a shows the largest supercell that we can study computationally. The distortions of the relaxed Nb surface with Mn in the optimal hollow position (see Supplementary Note 1; Materials and methods are available as supplementary materials at the npj Quantum Materials website) entail that the Nb(110) electronic structure with a Mn chain attached differs from the bulk band structure both because of surface relaxation and because of distortions due to the Mn chain. Figure 1b, d shows the fully relativistic (GGA+SO) spinpolarized band structure of our system, with Mn orbital character highlighted. We find that the ferromagnetic arrangement is 29.4 meV/Mn lower in energy than the antiferromagnetic one, indicating that Fig. 1b, d represents the DFT electronic ground state of the system. We find that an outofplane alignment of the magnetic moments is slightly lower in energy (by about 0.1 meV/Mn) compared to an inplane alignment. To construct a tightbinding model of the bandstructure obtained from the DFT calculations, we use projective Wannier functions within FPLO^{27}. However, the inclusion of all relevant orbitals, the Mn 3d, 4s, and 4p, as well as all Nb 4d, 5s, and 5d orbitals, would result in a 666 band tightbinding model, whose investigation, for example, in terms of the topological invariant or its realspace properties, is computationally beyond our current abilities. To arrive at a tractable tightbinding model, we therefore restrict our attention to the Mn 3d orbitals and the Nb 4d orbitals that bond with them (see highlighted Nb sites in Fig. 1a). This results in a 40band tight binding model, which (i) correctly reproduces the spectral weight of the Mn 3d bands (as given by the DFT results Fig. 1c, e), which are relevant for the emergence of topological superconductivity due to their magnetic moments, and (ii) contains the directiondependent d orbital overlaps as well as the effects of Mn spin splitting and Nb spin–orbit coupling.
80band model
We convert the DFTbased 40band tightbinding model into a superconducting 80band Bogoliubov–de Gennes model with the bare superconducting order parameter Δ as the only free parameter (see Supplementary Note 2). Note that we apply the superconducting onsite pairing term only to the orbitals of the three Nb atoms but not to the Mn atom; we assume that superconductivity is proximitized into the Mn orbitals, thus accurately describing the experimental system. It is important to emphasize that Δ here only serves as a phenomenological parameter and does not have a onetoone correspondence with the superconducting gap (which is known to be Δ_{Nb}=1.51 meV for Nb). In fact, it is quite clear that the bare Δ must be chosen to be much larger since the three Nb atoms represent the superconducting proximity effect of the entire (threedimensional) Nb substrate. In order to investigate the topological phase diagram of this model we compute the gap size and the topological invariant \({{{\mathcal{M}}}}\)^{1} characteristic of topological class D^{28,29}. The system is gapped, but the spectral gap is tiny for Δ < 130 meV (Fig. 2a) and ranges between 7 and 188 μeV for periodic boundary conditions (mean value 69 μeV). Moreover, we find for 0 < Δ < 120 meV and for Δ > 130 meV the ground state to be topologically nontrivial, i.e., \({{{\mathcal{M}}}}=1\) (Fig. 2a). Gap sizes for the regime Δ > 130 meV are in the range from 33 μeV to 1.83 meV (mean value 1.19 meV). Only the narrow region 120 meV < Δ < 130 meV turns out to be trivial. Our momentum space analysis thus reveals that Mn chains in the [001] direction on Nb(110) realize a topological superconductor, which due to bulkboundary correspondence is accompanied by MZMs that are localized at the chain ends. Chain length and effective gap size might, however, influence MZMs and cause them to hybridize in an oscillatory fashion as a function of length, which is one of the key signatures of hybridized MZMs in short chains^{30,31}.
Next, we study the realspace electronic structure, and in particular, that of the MZMs of the DFTbased 80band model. For short chains, it is very difficult to find localized zeroenergy states due to the tiny gap size leading to a severe hybridization of MZMs (Fig. 2b). Figure 2b reveals that there is no unique structure of MZMs, making it difficult to identify topological phases solely based on the spatial structure of the zeroenergy local density of states (LDOS). However, our computation of the topological invariant in real space^{32} shows that, as long as chains exceed ~10 sites, we find perfect agreement with our momentum space analysis shown in Fig. 2a. For Δ > 200 meV we find examples of zeroenergy LDOS where the hybridization leads to an oscillatory pattern and, quite astonishingly, the spectral weight of the MZMs is not located in the center of the chain but instead on the Nb atoms on the side of the magnetic chain. These side features show a striking similarity to recently reported scanning tunneling spectroscopy (STS) measurements on a Mn_{34} chain on Nb(110)^{20} (i.e., a chain consisting of 34 Mn atoms). We show in Fig. 2c three examples of the zeroenergy LDOS corresponding to different values of Δ and different chain lengths: a Mn_{34} chain with Δ = 320 meV (three maxima), a Mn_{51} chain with Δ = 300 meV (five maxima) and a Mn_{52} chain with Δ = 270 meV (six maxima). Their topological gap sizes for open boundary conditions are 3.10, 1.37, and 0.88 meV, respectively. We note that a selfconsistent treatment will typically suppress Δ near the magnetic chain, reducing the effective gap by a sizeable amount. This reduction can easily be as large as a factor of 3 or 4, which would bring the theoretical gap size to the same range as the experimental gap size of 180 μeV of one of the multiorbital YSRbands in the vicinity of the Mn[001] chains on Nb(110)^{20} (which is a factor of 8 smaller than the superconducting bulk gap, Δ_{Nb} = 1.51 meV). We emphasize that localization is governed by the coherence length, and thus longer chains lead to stronger localization of MZMs at the chain ends (see Supplementary Note 3.D). We note that side features can be observed for several values of Δ per chain length; we further note that MZMs can also appear in the chain center or combinations of side and center atoms (see for instance Supplementary Fig. 3). It turns out that contributions from different orbitals are sensitive to the chosen value of Δ, leading to a complex, nontrivial interplay of the five dorbitals in the lowenergy LDOS. All theoretical LDOS plots shown in the main text are purely twodimensional. In the Supplementary Note 4, we extend our analysis by including tip trajectory and tunneling geometry and show that the 3D LDOS still contains sides features; all our conclusions remain, hence, unchanged.
Throughout the manuscript, we use the term MZM for the lowenergy or zeroenergy states of the topological superconducting phase. The latter is determined by the topological invariant for both infinite and finite chains. Clearly, several of the considered examples of MZM are (strongly) hybridized, and in the literature alternative names such as ‘precursor of MZMs’ have been introduced^{31}. It is unknown whether hybridized MZMs are useful for braiding and thus for topological quantum computing, but that is not the topic of our paper. The aim of this paper is to demonstrate that a DFTbased modeling leads to a topological superconductor with lowenergy states which are exceedingly similar to what has been observed in the experiments.
Majorana zero modes with side features
In order to deepen our understanding of the side features in the zeroenergy LDOS, we analyze in the following a simplified model. Inspired by relevant orbitals of the 80band DFTbased model which lead to side features, we construct a oneorbital model which still has three “substrate” atoms carrying superconductivity and one magnetic atom (modeled by a Zeeman term), see Fig. 3a. We stress that the model still contains a nontrivial hopping structure which could not have been guessed by an ad hoc toy model; the multiband DFT input is key to derive and justify this ‘simplified’ model. We find for large gaps localized MZMs in the center of the chain ends (either on the magnetic or on the substrate atom), in agreement with previous modeling. However, when reducing the gap size (in an attempt to simulate the small experimental gap size), we find that the spectral weight of the MZMs drops to almost zero on the magnetic atoms. Moreover, spectral weight appears on the sideNb atoms, in agreement with the DFTbased model, reminiscent of previous experimental findings^{20}. A logical explanation for the formation of side features is as follows: the gap size corresponds to the strength of the superconductivity and thus to the proximity effect. In case of a large gap, i.e., of a significant superconducting proximity effect, superconductivity can be induced into the magnetic atoms and the MZM can be localized on the magnetic atoms at the chain ends. If the gap is small, however, the proximityinduced superconductivity competes with the magnetism of the Mn atoms, leading to suppressed superconducting correlations, and the MZMs are pushed away and localize along both sides instead.
The simplified model allows us to tune various parameters such as Rashba spin–orbit coupling, magnetic moment, chemical potential and superconducting pairing amplitude. We have analyzed the corresponding phase diagram and computed the fraction of the zeroenergy LDOS which is localized on the side next to the magnetic chain. 40 percent of the topological region of the phase diagram Fig. 3c turns out to exhibit notable side features, and ten percent of the examined parameter space possess 70–99 percent of the total spectral weight on the sides of the chain. We have also analyzed a variant of the model with an extended substrate in both x and y direction to rule out confinement effects perpendicular to the chain. We find that side features persist regardless of the size of the substrate or its boundary conditions (see Supplementary Note 3.F for details). These findings emphasize that side features in the lowenergy LDOS are not the exception but can be rather common. The oscillating behavior of the lowenergy modes is a more ordinary hybridization effect, which has previously been discussed in the context of other systems^{3,30,33,34,35}. We find that the smallest considered gap sizes lead to an equallydistributed pattern of oscillatory maxima along the chain (Fig. 3e, as found for the Mn_{51} chain in Fig. 2c). We also computed the evolution of sidefeature states with chain length N displaying an oscillatory behavior of the lowenergy states, see Fig. 3b.
When we slightly increase the gap size, these maxima disappear in the middle of the chain, but persist closer to the chain ends (an example with two such maxima at the chain ends is shown in Fig. 3f). Finally, we also find situations where MZMs are confined to the ends of the chains, still showing the side feature (Fig. 3g). We obtain a clear physical picture which emerges from our analysis: (i) when the substrate is included (via the three extra atoms per unit cell) and the gap is small, MZMs are forced to localize beside the magnetic chain on the substrate; (ii) for the smallest gap sizes considered, hybridization of MZMs is so strong that we obtain a periodic pattern of maxima in the zeroenergy LDOS [see Fig. 3d and e], as previously observed for the ab initio computed Mn_{51} chain in Fig. 2c and for a measured Mn_{34} chain in ref. ^{20}. This is in agreement with a very large coherence length ξ ~ v_{F}/Δ_{gap} exceeding the chain length (see Supplementary Note 3.D). Increasing the gap size reduces ξ and leads to a decaying envelope of the wavefunction, such that spectral weight in the bulk of the chain is suppressed.
Larger gap sizes result in even stronger localization of the MZMs (see Fig. 3g), showing a remarkable similarity to what was observed for an Fe chain on a Pb(110) substrate^{24}. We have computed coherence lengths and lowenergy LDOS for small, medium, and large gap sizes for extended parameter ranges, all in support of our previous conclusions (see Supplementary Notes 3.C and 3.D). While our ab initio model does not describe the Fe/Pb(110) system, we can still speculate that the topological lowenergy features might not depend on the specific system: there is clearly a strong similarity of the observed side feature with shorter coherence length (Fig. 3g) and the “double eye” seen in experiments^{24}. Due to the topological character we propose that the double eye feature found in Fe/Pb(110) has the same origin as the side features reported and modeled in this paper.
Experiment
To test the theoretical findings presented above, we studied linear chains of Mn and Fe assembled via lateral atom manipulation techniques on a clean Nb(110) surface^{20,31,36} (see refs. ^{20,31} and Supplementary Note 5 for details on sample preparation and chain construction). Figure 4a shows the topography of a Mn_{51} chain assembled along the [001] direction (upper panel), together with the spatial form of dI/dV for a state close to zero energy. The side features visible in dI/dV exhibit a close spatial similarity with those that exist in the theoretical LDOS shown in Figs. 2c and 3e (previously reported side features, such as those shown in Fig. 3 of ref. ^{20}, also exhibit a close similarity with Figs. 2c and 3d). The energy at which these side features are visible varies with the chain length N^{20}; the evolution of the side features’ energies with N is shown in Fig. 4b. Notably, the lowest energy state exhibiting these side features does not converge to E = 0 for chain lengths up to N = 36 but rather oscillates around zero energy. This result resembles the theoretical predictions shown in Fig. 3b (see also Supplementary Note 3.E) for a system with a small superconducting gap, and a chain length that is smaller than the coherence length. The combination of these two renders the experimental resolution of a topological gap exceedingly difficult. Indeed, our numerical simulations show that for the case shown in Fig. 3b, the chain length has to be significantly larger before a topological gap can be resolved and the Majorana mode is clearly separated from the bulk states.
To study the universality of the observed side features, we also investigated the lowenergy properties of a Fe_{16} chain along the [001] direction. This chain is structurally identical (see upper panel in Fig. 4c) to the Mn chains presented in Fig. 4a and ref. ^{20}, and predicted to have a ferromagnetic ground state as well^{26}. It also exhibits an enhanced zero energy dI/dV at both sides of the chain ends (lower panel in Fig. 4c). The notable similarity of these results with the theoretical calculations presented in Fig. 3f suggests a common origin of the side features observed for the Mn_{51} and Fe_{16} chains on Nb(110).
Discussion
The side features of the Mn chains were previously ascribed to bands formed by hybridization of Yu–Shiba–Rusinov (YSR) states of particular orbital character of the individual Mn impurities^{20,37}. Individual Fe atoms do not exhibit clear signatures of multiorbital YSR states^{38,39} (see Supplementary Note 6 for details), due to their close proximity to the coherence peaks of the substrate. Nevertheless, the linear Fe chains along the [001] direction, mentioned above, show an enhanced zeroenergy LDOS at the sides of both ends (Fig. 4c). This surprising observation, which cannot be explained by a linear combination of YSR states of the individual atoms (see Supplementary Note 6), shows obvious similarities with the theoretical calculations presented in Figs. 2c and 3. The interpretation of the observed side features as hybridized Majorana modes, as advocated in the theoretical part of this paper, is thus substantiated by the attempt to simultaneously explain the lowenergy features for Mn and Fe chains on Nb(110).
Motivated by our analysis relating these findings with the previously discovered doubleeye feature^{24}, we thus conclude that MZMs with side features might be a common phenomenon in MSH materials with small superconducting gap size. We note, however, counter examples do exist such as Fe/Re(0001)^{18,19} and Mn chains along [1\(\bar{1}\)0] on Nb(110)^{31}. This is, in fact consistent with our analysis of the superconducting 80band model: side features appear only for certain values of Δ, and changing Δ leads to a redistribution of the relative orbital weight. Since some of the Mn dorbitals support side features and others do not (see discussion of Supplementary Fig. 3), these ‘counter examples’ are compatible with the main results of our work. We emphasize that our results have farreaching consequences: the presence of pointlike zeroenergy modes at chain ends is considered as a necessary condition for the identification of onedimensional topological superconductors. Our work suggests that MZMs could, in fact, come in a large variety, ranging from delocalized, hybridized MZMs along the chain to localized MZMs on the chain. What determines whether a system is topological or not is not the spatial form of the lowest energy state, but the calculated value of the topological invariant. Our findings raise the important question whether MZMs with side features can be used for braiding and topological quantum computing, emphasizing the necessity to perform further theoretical and experimental work on onedimensional MSH structures.
Methods
Density functional theory calculations
We are using fully relativistic all electron DFT calculations based on the full potential local orbital (FPLO) basis^{40} in combination with a generalized gradient approximation (GGA) to the exchange correlation functional. We obtain low energy tight binding models using projective Wannier functions^{27}. The considered slab supercell is shown in Fig. 1a. We have fully relaxed the top half of the system while keeping the two bottom layers fixed at the Nb bulk lattice parameters and internal coordinates in order to simulate the experimental Nb(110) surface. We find that the top Nb layers contract slightly, lowering the nearest neighbor bond lengths. High symmetry positions for the placement of Mn are on top of Nb atoms and in the central hollow of the diamond arrangement of four Nb surface atoms. Energetically, the hollow position is 1.4 eV/Mn more favorable, in agreement with experimental observations and the calculations in ref. ^{37}. The Nb atoms forming bonds with Mn are measurably distorted out of their equilibrium Nb surface positions.
Superconducting 80band modeling
The projected 40band tightbinding model is given by
including essentially all possible hopping combinations up to fifth neighbors. Hopping amplitudes \({t}_{\sigma {\sigma }^{{\prime} }}^{i,o;j,{o}^{{\prime} }}\) are given as an input from DFT, and \({c}_{i,o,\sigma }^{{\dagger} }\) creates an electron with spin σ at orbital o at site i. We add the superconducting onsite pairing term \({H}_{\Delta }={\sum }_{i,o}\Delta {c}_{i,o,\uparrow }^{{\dagger} }{c}_{i,o,\downarrow }^{{\dagger} }+{{{\rm{H.c.}}}}\) and convert the model into an 80band Bogoliubovde Gennes model. As stressed before, the orbital index o only runs over the orbitals of the Nb atoms. We have calculated the topological invariant^{1} both in momentum and real space^{32} for this model. By virtue of Fourier transformation, we obtained the realspace representation, leading to matrix dimensions of 80N for chain length N, which can be diagonalized numerically. Open boundary conditions are enforced by setting all hopping amplitudes connecting the two chain ends to zero; to make the chain mirror symmetric, the central Nb atom is removed on the left side of the chain. In the Supplementary Note 3.F, we investigate finite chains embedded in a larger substrate in order to rule out edge and confinement effects.
Scanning tunneling microscopy and spectroscopy
The STM experiments were performed in a homebuilt UHV facility operated at a base temperature of T = 320 mK^{41}. The Nb(110) single crystal substrate was cleaned by high temperature flashes to T > 2700 K, following ref. ^{42}. Single Mn and Fe atoms were deposited onto the cold sample surface held at T < 7 K. A superconducting tip was prepared by indenting an electrochemically etched W tip into the substrate, thereby transferring large clusters of superconducting Nb onto the tip apex. STM topography images were measured in a constantcurrent mode with the current setpoint I while applying a constant bias voltage V_{DC} across the tunneling junction. Differential tunneling conductance (dI/dV) spectra were measured by stabilizing the tip at bias voltage V_{stab} and current I_{stab}. In the next step, the feedback loop was opened and V_{DC} was swept between −4 and +4 mV. The dI/dV signal was measured using a standard lockin technique with a small modulation voltage \({V}_{{{{\rm{mod}}}}}\) (RMS) of modulation frequency f = 4.142 kHz added to V_{DC}. The dI/dV maps were acquired by recording a set of dI/dV spectra on a rectangular grid. Superconducting Nb tips have been used in order to achieve a higher effective energy resolution. The measured differential tunneling conductance dI/dV is thus approximately proportional to a convolution of the LDOS of the sample and the superconducting tip density of states (DOS). We show numerically deconvoluted STS data throughout the manuscript, resembling the sample’s LDOS (see refs. ^{20,31} for details on the deconvolution process and determination of the tip gap). The Mn and Fe chains were assembled using lateral atom manipulation^{18,36,43} techniques at low tunneling resistances of R ≈ 12–60 kΩ.
Data availability
All data and materials needed to evaluate the conclusions in the paper are present in the paper and/or the Supplementary Information and are available for download at https://doi.org/10.5281/zenodo.6522954.
References
Kitaev, A. Y. Unpaired Majorana fermions in quantum wires. Phys.Usp. 44, 131–136 (2001).
Mourik, V. et al. Signatures of Majorana fermions in hybrid superconductorsemiconductor nanowire devices. Science 336, 1003–1007 (2012).
Albrecht, S. M. et al. Exponential protection of zero modes in Majorana islands. Nature 531, 206–209 (2016).
Deng, M. T. et al. Anomalous zerobias conductance peak in a NbInSb nanowireNb hybrid device. Nano Lett. 12, 6414–6419 (2012).
Ivanov, D. A. NonAbelian statistics of halfquantum vortices in pwave superconductors. Phys. Rev. Lett. 86, 268–271 (2001).
Nayak, C., Simon, S. H., Stern, A., Freedman, M. & Das Sarma, S. NonAbelian anyons and topological quantum computation. Rev. Mod. Phys. 80, 1083–1159 (2008).
Pientka, F., Glazman, L. I. & von Oppen, F. Topological superconducting phase in helical Shiba chains. Phys. Rev. B 88, 155420 (2013).
Li, J. et al. Topological superconductivity induced by ferromagnetic metal chains. Phys. Rev. B 90, 235433 (2014).
NadjPerge, S., Drozdov, I. K., Bernevig, B. A. & Yazdani, A. Proposal for realizing Majorana fermions in chains of magnetic atoms on a superconductor. Phys. Rev. B 88, 020407 (2013).
Schecter, M., Flensberg, K., Christensen, M. H., Andersen, B. M. & Paaske, J. Selforganized topological superconductivity in a Yu–Shiba–Rusinov chain. Phys. Rev. B 93, 140503 (2016).
Klinovaja, J., Stano, P., Yazdani, A. & Loss, D. Topological superconductivity and Majorana fermions in RKKY systems. Phys. Rev. Lett. 111, 186805 (2013).
Martin, I. & Morpurgo, A. F. Majorana fermions in superconducting helical magnets. Phys. Rev. B 85, 144505 (2012).
NadjPerge, S. et al. Observation of Majorana fermions in ferromagnetic atomic chains on a superconductor. Science 346, 602–607 (2014).
Ruby, M. et al. End states and subgap structure in proximitycoupled chains of magnetic adatoms. Phys. Rev. Lett. 115, 197204 (2015).
Pawlak, R. et al. Probing atomic structure and Majorana wavefunctions in monoatomic Fe chains on superconducting Pb surface. npj Quantum Inf. 2, 16035 (2016).
Jeon, S. et al. Distinguishing a Majorana zero mode using spinresolved measurements. Science 358, 772–776 (2017).
Ruby, M., Heinrich, B. W., Peng, Y., von Oppen, F. & Franke, K. J. Exploring a proximitycoupled Co chain on Pb(110) as a possible Majorana platform. Nano Lett. 17, 4473–4477 (2017).
Kim, H. et al. Toward tailoring Majorana bound states in artificially constructed magnetic atom chains on elemental superconductors. Sci. Adv. 4, eaar5251 (2018).
Schneider, L. et al. Controlling ingap end states by linking nonmagnetic atoms and artificiallyconstructed spin chains on superconductors. Nat. Commun. 11, 4707 (2020).
Schneider, L. et al. Topological Shiba bands in artificial spin chains on superconductors. Nat. Phys. 17, 943–948 (2021).
Choy, T.P., Edge, J. M., Akhmerov, A. R. & Beenakker, C. W. J. Majorana fermions emerging from magnetic nanoparticles on a superconductor without spin–orbit coupling. Phys. Rev. B 84, 195442 (2011).
Crawford, D., Mascot, E., Morr, D. K. & Rachel, S. Hightemperature Majorana fermions in magnetsuperconductor hybrid systems. Phys. Rev. B 101, 174510 (2020).
Mier, C., Choi, D.J. & Lorente, N. Calculations of ingap states of ferromagnetic spin chains on swave wideband superconductors. Phys. Rev. B 104, 245415 (2021).
Feldman, B. E. et al. Highresolution studies of the Majorana atomic chain platform. Nat. Phys. 13, 286–291 (2017).
Kobiałka, A., Piekarz, P., Oleś, A. M. & Ptok, A. Firstprinciples study of the nontrivial topological phase in chains of 3d transition metals. Phys. Rev. B 101, 205143 (2020).
Laszloffy, A., Palotas, K., Rozsa, L. & Szunyogh, L. Electronic and magnetic properties of building blocks of Mn and Fe atomic chains on Nb(110). Nanomaterials 11, 1933 (2021).
Eschrig, H. & Koepernik, K. Tightbinding models for the ironbased superconductors. Phys. Rev. B 80, 104503 (2009).
Kitaev, A. Periodic table for topological insulators and superconductors. AIP Conf. Proc. 22, 1134 (2009).
Schnyder, A. P., Ryu, S., Furusaki, A. & Ludwig, A. W. W. Classification of topological insulators and superconductors in three spatial dimensions. Phys. Rev. B 78, 195125 (2008).
Stanescu, T. D., Lutchyn, R. M. & Sarma, S. D. Dimensional crossover in spin–orbitcoupled semiconductor nanowires with induced superconducting pairing. Phys. Rev. B 87, 094518 (2013).
Schneider, L. et al. Precursors of Majorana modes and their lengthdependent energy oscillations probed at both ends of atomic Shiba chains. Nat. Nanotechnol. 17, 384–389 (2022).
Budich, J. C. & Ardonne, E. Equivalent topological invariants for onedimensional Majorana wires in symmetry class D. Phys. Rev. B 88, 075419 (2013).
Klinovaja, J. & Loss, D. Composite Majorana fermion wave functions in nanowires. Phys. Rev. B 86, 085408 (2012).
Deng, M. T. et al. Majorana bound state in a coupled quantumdot hybridnanowire system. Science 354, 1557–1562 (2016).
Deng, M. T. et al. Nonlocality of Majorana modes in hybrid nanowires. Phys. Rev. B 98, 085125 (2018).
Schneider, L., Beck, P., Wiebe, J. & Wiesendanger, R. Atomicscale spinpolarization maps using functionalized superconducting probes. Sci. Adv. 7, eabd7302 (2021).
Beck, P. et al. Spin–orbit coupling induced splitting of Yu–Shiba–Rusinov states in antiferromagnetic dimers. Nat. Commun. 12, 2040 (2021).
Odobesko, A. B. et al. Observation of tunable singleatom Yu–Shiba–Rusinov states. Phys. Rev. B 102, 174504 (2020).
Küster, F. et al. Correlating Josephson supercurrents and Shiba states in quantum spins unconventionally coupled to superconductors. Nat. Commun. 12, 1108 (2021).
Koepernik, K. & Eschrig, H. Fullpotential nonorthogonal localorbital minimumbasis bandstructure scheme. Phys. Rev. B 59, 1743–1757 (1999).
Wiebe, J. et al. A 300 mK ultrahigh vacuum scanning tunneling microscope for spinresolved spectroscopy at high energy resolution. Rev. Sci. Instrum. 75, 4871–4879 (2004).
Odobesko, A. B. et al. Preparation and electronic properties of clean superconducting Nb(110) surfaces. Phys. Rev. B 99, 115437 (2019).
Eigler, D. M. & Schweizer, E. K. Positioning single atoms with a scanning tunnelling microscope. Nature 344, 524–526 (1990).
Acknowledgements
The authors acknowledge discussions and previous collaborations with L. Schneider. J.W. and R.W. gratefully acknowledge funding by the Cluster of Excellence ‘Advanced Imaging of Matter’ (EXC 2056  project ID 390715994) of the Deutsche Forschungsgemeinschaft (DFG). P.B., J.W., and R.W. acknowledge support by the DFG via SFB 925  project ID 170620586. R.W. gratefully acknowledges financial support from the European Union via the ERC Advanced Grant ADMIRE (project No. 786020). M.S. acknowledges support by GrantinAid for JSPS Fellows No. JP21J12095. E.M. and D.K.M. acknowledge support from the U. S. Department of Energy, Office of Science, Basic Energy Sciences, under Award No. DEFG0205ER46225. S.R. acknowledges support from the Australian Research Council through Grant No. DP200101118.
Author information
Authors and Affiliations
Contributions
M.S. and H.O.J. performed the DFT calculations and derived the 40band tightbinding model. D.C., E.M., D.K.M., and S.R. performed all other theoretical modeling. P.B., R.W., and J.W. conceived the experiments. P.B. performed the measurements and analyzed the experimental data together with J.W. S.R. wrote the manuscript, with contributions from all authors. All authors contributed to the discussions and to correcting the manuscript.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Supplementary information
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Crawford, D., Mascot, E., Shimizu, M. et al. Majorana modes with side features in magnetsuperconductor hybrid systems. npj Quantum Mater. 7, 117 (2022). https://doi.org/10.1038/s4153502200530x
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s4153502200530x
This article is cited by

Majorana zero modes in Yshape interacting Kitaev wires
npj Quantum Materials (2023)

Probing the topologically trivial nature of end states in antiferromagnetic atomic chains on superconductors
Nature Communications (2023)